conversion and leaching characteristics of biomass ashes ... ?· conversion and leaching...
Post on 23-Jul-2018
Embed Size (px)
Conversion and leaching characteristics of biomass ashes during outdoor storage Dipl.-Ing. Klaus Supancic1,*, Prof. Univ.-Doz. Dipl.-Ing. Dr. Ingwald Obernberger1,2,3, Dipl.-Ing. Norbert Kienzl3, Ing. Anton Arich3 1 BIOS BIOENERGIESYSTEME GmbH, Inffeldgasse 21b, A-8010 Graz, Austria, www.bios-bioenergy.at *Corresponding author: e-mail firstname.lastname@example.org 2 Institute of Process and Particle Engineering Graz University of Technology, Inffeldgasse 13/III, A-8010 Graz, Austria 3 BIOENERGY 2020+ GmbH, Inffeldgasse 21b, A-8010 Graz, Austria
Introduction and objectives In recent years, the promotion of energy production from biomass in Austria and the European Union has led to a strong increase in the amount of combustion residues, i.e. ashes. Finding ways to utilize these ashes in an environmentally and economically efficient manner is thus an important goal throughout Europe. The utilization of the nutrient rich and rather heavy metal poor wood ash fractions (bottom and coarse fly ash) for fertilizing and soil improvement purposes is already implemented in Austria and several European countries (Sweden, Finland and Germany to name a few). The utilization path, however, implicates logistic challenges for many biomass plant operators, since the main part of the ash is often produced during the winter season whereas ash application usually takes place during warmer periods. Therefore, a logistic concept considering intermediate storage sites is necessary. As the ash has to be stored for several months, it seems reasonable to take advantage of the storage period and facilitate the self-hardening process by adding water . The most important reaction of the hardening process is the transformation of CaO to Ca(OH)2 and further into CaCO3 which lowers the calcium leaching rate significantly and leads to a reduction of the pH-level. Alkaline shock effects on ground vegetation can thus be prevented. In December 2009, a 4-year R&D-project was initiated in Austria with the focus on the development of innovative strategies of ash utilization in order to promote increased ash utilization. The improvement of ash logistics with a detailed investigation of intermediate outdoor storage of wood ashes in order to provide biomass plant operators with guidelines for proper intermediate ash storage is one of the main topics of this project. Background The intermediate outdoor storage of wood ash is especially relevant if the wood ash shall be used as a fertilizing and liming agent in agriculture and forestry. Usually the main part of the ash is often produced during the winter season whereas ash application on agricultural and forest soils is not allowed before spring. Since the storage capacities at biomass plants are limited, the ash produced during winter needs to be stored on storage areas outside the biomass plant premises. If possible, the storage area should be located close to the agricultural or forest areas where the ash application is planned, in order to reduce transport routes and thus minimizing the lag time between filling of the spreading device and ash application . Due to the chemical composition of wood ash, which contains up to up to 50 % mass fraction of CaO in the dry material, the addition of water facilitates the formation of Ca(OH)2 and further with airborne CO2 the formation of CaCO3 (carbonatation). This process changes the chemical and physical properties of the ash and leads to self-hardening. Practical experience from Sweden [1, 2, 3, 4], where self-hardening is recommended for biomass ash utilization in forests since it reduces the pH-level (negative effects on ground vegetation caused by alkali burn can be prevented) as well as the dust formation of biomass ashes, shows that by adding a specific amount of water the carbonatation process can be improved. The carbonatation of biomass ashes also leads to a reduced leaching of Ca, thus a longer lasting liming effect of the ash can be achieved. However, intermediate outdoor storage of ashes is only reasonable, if negative ecological effects like dust formation and leaching of heavy metals and other hazardous compounds can be avoided. Therefore, a detailed investigation of the ecological effects of intermediate outdoor storage is necessary. In addition, the optimum water mixing rates for self-hardening shall be determined. Methodology The research and development activities followed a three-step-approach:
1. Performance of laboratory tests with ash samples from different combustion technologies (fluidized and fixed bed combustion) over 16 weeks in order to determine the changes of the
ash quality and the leaching behavior depending on the duration of the storage and the amount of water added to the ash (performed 2010).
2. Performance of field tests with ashes from the same combustion technologies over 6 months. During the tests, leachate from the storage sites was sampled and analyzed in regular intervals. In addition, the ash itself was sampled and analyzed regularly (performed 2011).
3. Performance of additional laboratory tests with bottom ash from a grate furnace and coarse fly ash from a bubbling fluidized bed furnace over 16 weeks in order to determine the optimal water mixing rate for the ageing of ashes during storage (performed 2013).
The storage conditions applied in the respective tests are shown in Table 1.
Table 1: Storage conditions applied in the individual storage tests Explanations: GF grate furnace; BFBF bubbling fluidised bed furnace; CFBF circulating fluidised bed furnace
1st laboratory tests Field tests 2nd laboratory testsStorage period 16 weeks 24 weeks 16 weeksAshes investigated 1) bottom ash from a GF fired with bark and wood
chips,2) mixture of bottom ash and coarse fly ash from a GF fired with bark and wood chips,3) boiler fly ash from a BFBF fired with wood chips, 4) fine bottom ash from a CFBF fired with forest residues
1) bottom ash from a GF fired with bark and wood chips,2) mixture of bottom ash and coarse fly ash from a GF fired with bark and wood chips,3) boiler fly ash from a BFBF fired with wood chips, 4) bottom ash from a GF fired with bark
1) bottom ash from a GF fired with bark and wood chips,2) boiler fly ash from a BFBF fired with wood chips
Storage conditions 1 open dry sample per ash (all ashes)2 open wet samples per ash (all ashes)2 airtight wet samples (bottom ash from a GF and coarse fly ash from a BFBF only)Regular wetting of the samples with a water sprayer
Ashes 1) to 3) were delivered dry, ash 4) was delivered in wet condition (24% water mass fraction, wet basis).3 piles per ash, each pile was sprinkled with water corresponding to 40 mm/m of rainfall at the beginning of the storage period. Natural rainfall during storage
1 open dry sample per ash (all ashes)3 open wet samples per ash (all ashes)Regular wetting of the samples with a water sprayer
Sampling after 1, 2, 4, 8 and 16 weeks after 1, 2, 4, 8, 12, 16, 20 and 24 weeks, sampling of the outside layer and the inner zone;Collection and sampling of leachate and rainwater as a reference
after 1, 4, 8 and 16 weeks
Water mixing rates Ash 1) and 2): 16.7 and 27.0% (water mass fraction, wet basis),ash 3) 15.3 and 21.9% (water mass fraction, wet basis),ash 4) 17.4% (water mass fraction, wet basis)
Sprinkling with water at the beginning of the tests, some 250 mm/m rainfall over 24 weeks
Ash 1): 9.7, 12.6 and 15.1% (water mass fraction, wet basis),ash 2): 4.5, 5.9 and 7.3% (water mass fraction, wet basis)
Laboratory tests The purpose of the laboratory tests performed in 2010 was the investigation of the conversion and leaching behavior of different wood ash fractions (bottom ash and mixture of bottom ash and coarse fly ash from a grate furnace (GF) fired with bark and wood chips, boiler fly ash from a bubbling fluidized bed furnace (BFBF) fired with wood chips, fine bottom ash from a circulating fluidized bed furnace (CFBF) fired with forest residues under different storage conditions (dry/wet, open or in absence of air). The results of the laboratory tests shall also be used to pre-evaluate the ecological impact of ash storage (leaching behavior) as well as its impact on the quality of the ash stored (self-hardening) and provide the basis for the design of the outdoor storage tests which were performed from April to October 2011. At the beginning of the storage test the four ash fractions selected (original samples) were physically (particle size distribution) and chemically (water mass fraction, CaO mass fraction, TIC mass fraction, pH-level, electrical conductivity, chemical composition, leaching ratio of major elements as well as heavy metals), characterized. In detail, the following elements were analyzed in the solid matter: Si, Ca, Mg, K, Na, P, Al, Fe, Mn, As, Cd, Co, Cr, Cu, Mo, Ni, Pb, V, Zn, S, Cl. The following elements were analyzed in the leachate: Cr (VI), Cl, S, Si, Ca, Mg, K, Na, P, Al, Fe, Mn, Cu, Zn, Co, Mo, Ni, Cr, Pb and Cd. In addition, the main crystalline components were analyzed using X-ray diffraction. For each ash fraction dry and wet samples were stored over a period of 16 weeks. The amount of water added was estimated based on the experience of earlier tests performed in Sweden (the amount of water required for hardening was estimated based on the content of CaO and other components that may take up water) as well as on the results of preliminary tests performed prior to the lab-test. Based on these findings two different water mixing rates were defined for the two ash fractions from the grate furnace and the boiler fly ash from the BFBF. Since the content of CaO and other components that can form hydrates of the fine bottom ash from a CFBF is due to the dilution with bed material (SiO2) very low, only one water mixing rate was determined. In order to avoid the